Structural, Optical and Electrical Properties of Undoped and Doped ZnO Thin Films

Lourdhu Bruno Chandrasekar, S. Nagarajan, Marimuthu Karunakaran and T. Daniel Thangadurai

### Abstract

ZnO, which has high electrochemical stability, wide band gap energy, large excitonic binding energy, intense near band excitonic emission and is non-toxic, have potential applications in all fields. This chapter reviews the structural, optical and electrical properties of undoped and doped ZnO thin films. The type of doping highly influences the structural properties such as grain size, texture coefficient and unit cell properties. The dopants of transition metal and nonmetals have unique characteristics. Moreover, mono-doping and co-doping encourage this research. The optical properties such as bandgap, charge carrier concentrations and transmissions of the films depend on the doping as well as the preparation condition of the films. The effect of doping on its properties is also discussed.

Keywords: structural, electrical, ZnO, doping

### 1. Introduction

Recent developments in low-dimensional semiconductors create a wide range of applications and opportunities for the fabrication of varieties of devices for the future. The confinement of the charge carrier results in providing unique properties to the materials which are size dependent. Transparent conducting oxides such as CuO, Sn2O and ZnO have potential applications in the field of photovoltaic and sensing systems. Out of many transparent conducting oxides, ZnO has unique properties such as high excitation binding energy at room temperature, chemical and thermal stability, n-type semiconductor, biocompatibility, etc. [1, 2]. They have a wide range of applications including antibacterial activity, photodetectors, memory applications, LED, solar cell, gas sensors and acoustic wave devices [3–11]. The interests in the ZnO thin films can be viewed easily by the millions of research articles on ZnO thin films prepared under different conditions like substrate temperature, pH value of the solution, doping concentration and annealing temperature. Spray pyrolysis, successive ionic layer adsorption and reaction (SILAR), magnetron sputtering, sol-gel spin coating, pulsed laser deposition, atomic layer deposition and chemical bath deposition are some of the few methods available to prepare the undoped and doped ZnO films [10, 12–17]. Recently, co-doped ZnO such as Al-In-doped ZnO films and F-In-doped ZnO films, ZnO-based thin film transistors, field emission display, white light emission and p-type ZnO encourage

**16**

*2D Materials*

**References**

physics/1985/summary

physics/1998/summary

physics/2010/press-release

2011

2011

[1] Nobelprize.org Physics Prize (1985) [Internet]. 2018. Available from: https://www.nobelprize.org/prizes/

[10] Cunha E, Ren H, Lin F, Kinloch IA, Sun Q, Fan Z, et al. The chemical functionalization of graphene nanoplatelets through solvent-free reaction. Royal Society of Chemistry Advances. 2018;**8**:33564-33572

[11] Hodkiewicz J. Characterizing carbon materials with Raman spectroscopy. Thermo-Fisher Scientific Application

[12] Tuinstra F, Koenig JL. Raman spectrum of graphite. The Journal of Chemical Physics. 1970;**53**(3):1126-1130

[13] Cancado LG, Takai K, Enoki T, Endo M, Kim YA, Mizuasaki H, et al. Measuring the degree of stacking order in graphite by Raman spectroscopy.

[14] Wojdyr M. Fityk a general-purpose peak fitting program. Journal of Applied Crystallography. 2010;**43**:1126-1128

Carbon. 2008;**46**:272-275

Note. 2010;**51901**:1-5

[2] Nobelprize.org Physics Prize (1998) [Internet]. 2018. Available from: https://www.nobelprize.org/prizes/

[3] Nobelprize.org Physics Prize (2010) [Internet]. 2018. Available from: https://www.nobelprize.org/prizes/

[4] Wong HSP, Akinwande D. Carbon Nanotube and Graphene Device Physics. New York: Cambridge University Press;

[5] Jorio A, Saito R, Dresselhaus G, Dresselhaus M. Raman Spectroscopy in Graphene Related Systems. Weinheim: Wiley-VCH Verlag GmbH & Co. KGaA;

[6] STREM Graphene Nanoplatelets Data Sheet [Internet]. Available from: https://secure.strem.com/uploads/ resources/documents/graphene\_

[7] Graphene Supermarket Fluorinated Graphene Nanoplatelets Data [Internet].

Available from: https://graphenesupermarket.com/Fluorinated-Graphene-Nanoplatelets.html

[8] Binning G, Rohrer H, Gerber C, Weibel E. Surface studies by scanning tunneling microscopy. Physical Review

[9] Chieng WB, Ibrahim NA, Yunus WMZW, Hussein MZ, Then YY, Loo YY. Effects of graphene nanoplatelets and reduced graphene oxide on poly(lactic acid) and plasticized poly (lactic acid): A comparative study. Polymers.

nanoplatelets\_copy1.pdf

Letters. 1982;**49**:57

2014;**6**:2232-2246

became dominant than (102), (110) and (103) which are dominant for the pristine system. The doping concentration influences the relative intensity observed between the planes (100), (002) and (101). The intensity of (100) peak is maximum when the doping concentration is 0%, and the intensity of (101) peak enhances than (100) peak when the doping concentration is 4%. The variation has been speculated. Nonsystematic variation of grain size is observed as a function of doping concentration. This is because of the fact that the grain size not only depends on the doping concentration but also depends on the crystallographic axes. The packing fraction decreases from 1.612 to 1.602 as the doping concentration increases from 0 to 4% (atomic doping concentration). Figure 2 shows the grain size and the packing fraction of Co-doped ZnO thin film as a function of Co doping concentration.

Structural, Optical and Electrical Properties of Undoped and Doped ZnO Thin Films

Singh et al. reported the Fe- and Ge-doped ZnO thin films prepared by pulsed laser deposition method [25]. The undoped and doped ZnO (Zn0.98Ga0.02O and Zn0.98Fe0.02O) thin films show a strong reflection from (002) plane. The grain size corresponds to this miller plane and increases when Ga is doped, and the same decreases when Fe is doped, compared with the undoped ZnO. Moreover, Ga doping increases the texture of the material but decreases the c-lattice parameter. But this situation is reversed due to the doping of Fe. That is, the doping of Fe in ZnO deteriorates the crystalline nature of the material and the c-lattice parameter increases. The same result is obtained when yttrium (Y) is doped in ZnO thin film prepared by sol-gel technique [26]. The reason is due to the fact that ionic radii of Fe2+ and Y3+ are greater than the ionic radii of Zn2+. In both cases, the addition of either Fe or Y ion shifts the (002) miller plane to the lower angle side. The doping of Y3+ in Zn2+ lattice increases the c-lattice parameter from 5.205 to 5.247 Å linearly as

The effect of Ni doping in ZnO thin film is reported by Yilmaz [27]. All the films have c-axis orientation which is confirmed by the (002) peaks. The intensity of (002) peak decreases when the doping concentration of Ni increases. The lattice constants are nearly equal irrespective of Ni doping. The full-width at half-maximum (FWHM) increases from 0.266 to 0.344° which indicates that the grain size decreases as the doping of Ni increases. Figure 3 shows the Ni doping concentration vs. the full-width at half-maximum of the maximum intensity peak. Figures 4 and 5 indicate the grain size and the dislocation density of the prepared films as a function of doping. The results clearly indicate that the microstructural properties of Ni-doped ZnO thin films

the function of doping concentration.

DOI: http://dx.doi.org/10.5772/intechopen.88905

Figure 2.

19

are highly influenced by the doping concentration.

'Co' doping concentration vs. grain size and packing fraction.

this research [18–22]. This chapter provides an insight into the structural, optical and electrical properties of undoped and doped wurtzite geometry ZnO thin films which are quite important for future potential device designs. Figure 1 shows the representation of wurtzite geometry ZnO. The lattice constants 'a' and 'c' are related by the d-spacing of the corresponding Miller indices (hkl) by <sup>d</sup>�<sup>2</sup> <sup>¼</sup> <sup>4</sup> 3 h2 þhkþk<sup>2</sup> a2 � � <sup>þ</sup> <sup>l</sup> 2 <sup>c</sup>2. The ideal value of lattice constants 'a' and 'c' are, respectively, 0.325 and 0.521 nm. The bond length is calculated as b ¼ ffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffi 1 <sup>3</sup> a<sup>2</sup> þ ð Þ 0:5 � u 2 c2 q , where u is 0.25 + {0.33a<sup>2</sup> /c 2 }. The bond angles are <sup>α</sup> <sup>¼</sup> <sup>π</sup> <sup>2</sup> þ arccos ffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffi <sup>1</sup> <sup>þ</sup> <sup>3</sup>ð Þ <sup>c</sup>=<sup>a</sup> <sup>2</sup> ð Þ <sup>0</sup>:<sup>5</sup> � <sup>u</sup> <sup>2</sup> � � <sup>q</sup> �<sup>1</sup> " # and β ¼ 2 arcsin ffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffi 4 <sup>3</sup> þ 4ð Þ c=a <sup>2</sup> ð Þ <sup>0</sup>:<sup>5</sup> � <sup>u</sup> 2 � � <sup>q</sup> �<sup>1</sup> " # [23, 24]. It has 3.37 eV band gap at

room temperature and possesses both paramagnetic and ferromagnetic nature according to the type of doping.

The structural properties of the ZnO thin films are seldom affected during doping up to certain atomic concentrations, and the structure gets modified slightly due to doping. The structural properties of the doped ZnO thin films are given in Section 2. The changes in optical properties, mainly the band gap variation, are discussed in Section 3. The variations in electrical properties of the undoped and doped thin films are presented in Section 4 followed by the conclusion.

#### 2. Structural properties

Co-doped ZnO thin film is used in transparent electrode applications, where indium-tin-oxide was used in the past. For example, spray pyrolysis is employed to prepare the Co-doped ZnO thin film, and the structural properties are analysed with different doping concentrations [1]. The XRD studies reveal that the wurtzite nature of the materials is retained. The Miller indices (100), (002) and (101)

#### Structural, Optical and Electrical Properties of Undoped and Doped ZnO Thin Films DOI: http://dx.doi.org/10.5772/intechopen.88905

became dominant than (102), (110) and (103) which are dominant for the pristine system. The doping concentration influences the relative intensity observed between the planes (100), (002) and (101). The intensity of (100) peak is maximum when the doping concentration is 0%, and the intensity of (101) peak enhances than (100) peak when the doping concentration is 4%. The variation has been speculated. Nonsystematic variation of grain size is observed as a function of doping concentration. This is because of the fact that the grain size not only depends on the doping concentration but also depends on the crystallographic axes. The packing fraction decreases from 1.612 to 1.602 as the doping concentration increases from 0 to 4% (atomic doping concentration). Figure 2 shows the grain size and the packing fraction of Co-doped ZnO thin film as a function of Co doping concentration.

Singh et al. reported the Fe- and Ge-doped ZnO thin films prepared by pulsed laser deposition method [25]. The undoped and doped ZnO (Zn0.98Ga0.02O and Zn0.98Fe0.02O) thin films show a strong reflection from (002) plane. The grain size corresponds to this miller plane and increases when Ga is doped, and the same decreases when Fe is doped, compared with the undoped ZnO. Moreover, Ga doping increases the texture of the material but decreases the c-lattice parameter. But this situation is reversed due to the doping of Fe. That is, the doping of Fe in ZnO deteriorates the crystalline nature of the material and the c-lattice parameter increases. The same result is obtained when yttrium (Y) is doped in ZnO thin film prepared by sol-gel technique [26]. The reason is due to the fact that ionic radii of Fe2+ and Y3+ are greater than the ionic radii of Zn2+. In both cases, the addition of either Fe or Y ion shifts the (002) miller plane to the lower angle side. The doping of Y3+ in Zn2+ lattice increases the c-lattice parameter from 5.205 to 5.247 Å linearly as the function of doping concentration.

The effect of Ni doping in ZnO thin film is reported by Yilmaz [27]. All the films have c-axis orientation which is confirmed by the (002) peaks. The intensity of (002) peak decreases when the doping concentration of Ni increases. The lattice constants are nearly equal irrespective of Ni doping. The full-width at half-maximum (FWHM) increases from 0.266 to 0.344° which indicates that the grain size decreases as the doping of Ni increases. Figure 3 shows the Ni doping concentration vs. the full-width at half-maximum of the maximum intensity peak. Figures 4 and 5 indicate the grain size and the dislocation density of the prepared films as a function of doping. The results clearly indicate that the microstructural properties of Ni-doped ZnO thin films are highly influenced by the doping concentration.

Figure 2. 'Co' doping concentration vs. grain size and packing fraction.

this research [18–22]. This chapter provides an insight into the structural, optical and electrical properties of undoped and doped wurtzite geometry ZnO thin films which are quite important for future potential device designs. Figure 1 shows the representation of wurtzite geometry ZnO. The lattice constants 'a' and 'c'

<sup>c</sup>2. The ideal value of lattice constants 'a' and 'c' are, respectively,

<sup>2</sup> þ arccos

1

q

ffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffi

ffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffi <sup>1</sup> <sup>þ</sup> <sup>3</sup>ð Þ <sup>c</sup>=<sup>a</sup> <sup>2</sup> ð Þ <sup>0</sup>:<sup>5</sup> � <sup>u</sup> <sup>2</sup> � � <sup>q</sup> �<sup>1</sup> " #

2 c2

, where

<sup>3</sup> a<sup>2</sup> þ ð Þ 0:5 � u

[23, 24]. It has 3.37 eV band gap at

are related by the d-spacing of the corresponding Miller indices (hkl) by

}. The bond angles are <sup>α</sup> <sup>¼</sup> <sup>π</sup>

ffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffi

� � <sup>q</sup> �<sup>1</sup> " #

<sup>2</sup> ð Þ <sup>0</sup>:<sup>5</sup> � <sup>u</sup>

doped thin films are presented in Section 4 followed by the conclusion.

room temperature and possesses both paramagnetic and ferromagnetic nature

The structural properties of the ZnO thin films are seldom affected during doping up to certain atomic concentrations, and the structure gets modified slightly due to doping. The structural properties of the doped ZnO thin films are given in Section 2. The changes in optical properties, mainly the band gap variation, are discussed in Section 3. The variations in electrical properties of the undoped and

Co-doped ZnO thin film is used in transparent electrode applications, where indium-tin-oxide was used in the past. For example, spray pyrolysis is employed to prepare the Co-doped ZnO thin film, and the structural properties are analysed with different doping concentrations [1]. The XRD studies reveal that the wurtzite nature of the materials is retained. The Miller indices (100), (002) and (101)

2

<sup>d</sup>�<sup>2</sup> <sup>¼</sup> <sup>4</sup> 3 h2 þhkþk<sup>2</sup> a2 � �

Figure 1.

2D Materials

u is 0.25 + {0.33a<sup>2</sup>

and β ¼ 2 arcsin

þ l 2

Representation of wurtzite geometry ZnO unit cell.

/c 2

according to the type of doping.

2. Structural properties

18

4

0.325 and 0.521 nm. The bond length is calculated as b ¼

<sup>3</sup> þ 4ð Þ c=a

Figure 3. 'Ni' doping concentration vs. FWHM.

preferred orientation for the undoped ZnO film is 0.18°, and it is 0.21° for Al-doped ZnO films. It is clear evidence that the average grain size decreases from 46 to 39 nm due to the doping of Al. This is due to the contraction of the unit cell and Zn ions which have radius 0.74 Å is replaced by the Al ions (radius 0.51 Å). The absence of the peak (103) in the undoped sample becomes considered as the doping concentration increases. This kind of results is reported in Sr-doped ZnO thin films [16]. The grain size changes from 82 to 28 nm when the ZnO is doped with Sr. In the Al-doped ZnO films, which are prepared by sol-gel dip coating method, the peak (002) is dominant and becomes more dominant as the concentration of Al increases, but the intensity of the peak deteriorates when 'Al' concentration

Structural, Optical and Electrical Properties of Undoped and Doped ZnO Thin Films

The position of the peak (002) shifts to a lower angle side as the doping concentration increases, and it is shown in Figure 6. The peak (103) is dominant in the

becomes 10% [30].

Figure 6.

21

'Al' doping concentration vs. peak position.

Figure 5.

'Ni' doping concentration vs. dislocation density.

DOI: http://dx.doi.org/10.5772/intechopen.88905

Figure 4. 'Ni' doping concentration vs. grain size.

Ni-doped ZnO thin films are prepared by a modified SILAR method and are reported by Karunakaran et al. [28]. The microstructural properties are analysed as a function of the concentration of nickel sulphate (source material for nickel) and the annealing temperature of the films. As the nickel sulphate concentration changes from 5 to 10 mM, the grain size increases from 29.5 to 44.6 nm. The miller plane (002) has high intensity when the concentration of nickel sulphate is 5 and 10 mM. However, the dominant peak orientation shifts from (002) plane to (101) plane with concentration 15 mM. The annealing increases the crystalline size of the films. The as-deposited films have the average grain size of 45.2 nm, whereas the average grain size is 48.2, 49.7 and 52.8 nm when the films are annealed at 200, 300 and 400°C for 60 min in air, respectively.

Al-doped ZnO thin films, which are prepared by SILAR method, show a redshift towards a higher diffraction angle in the XRD pattern [29]. The line width of the

Structural, Optical and Electrical Properties of Undoped and Doped ZnO Thin Films DOI: http://dx.doi.org/10.5772/intechopen.88905

Figure 5. 'Ni' doping concentration vs. dislocation density.

preferred orientation for the undoped ZnO film is 0.18°, and it is 0.21° for Al-doped ZnO films. It is clear evidence that the average grain size decreases from 46 to 39 nm due to the doping of Al. This is due to the contraction of the unit cell and Zn ions which have radius 0.74 Å is replaced by the Al ions (radius 0.51 Å). The absence of the peak (103) in the undoped sample becomes considered as the doping concentration increases. This kind of results is reported in Sr-doped ZnO thin films [16]. The grain size changes from 82 to 28 nm when the ZnO is doped with Sr. In the Al-doped ZnO films, which are prepared by sol-gel dip coating method, the peak (002) is dominant and becomes more dominant as the concentration of Al increases, but the intensity of the peak deteriorates when 'Al' concentration becomes 10% [30].

The position of the peak (002) shifts to a lower angle side as the doping concentration increases, and it is shown in Figure 6. The peak (103) is dominant in the

Figure 6. 'Al' doping concentration vs. peak position.

Ni-doped ZnO thin films are prepared by a modified SILAR method and are reported by Karunakaran et al. [28]. The microstructural properties are analysed as a function of the concentration of nickel sulphate (source material for nickel) and the annealing temperature of the films. As the nickel sulphate concentration changes from 5 to 10 mM, the grain size increases from 29.5 to 44.6 nm. The miller plane (002) has high intensity when the concentration of nickel sulphate is 5 and 10 mM. However, the dominant peak orientation shifts from (002) plane to (101) plane with concentration 15 mM. The annealing increases the crystalline size of the films. The as-deposited films have the average grain size of 45.2 nm, whereas the average grain size is 48.2, 49.7 and 52.8 nm when the films are annealed at 200, 300

Al-doped ZnO thin films, which are prepared by SILAR method, show a redshift towards a higher diffraction angle in the XRD pattern [29]. The line width of the

and 400°C for 60 min in air, respectively.

Figure 3.

2D Materials

Figure 4.

20

'Ni' doping concentration vs. FWHM.

'Ni' doping concentration vs. grain size.


to the band gap 3.3 eV, 'band edge' excitonic states and reflections of the secondorder harmonic of the excitation source, respectively. Apart from the second-order harmonic peak, the peak 'band edge' excitonic state is dominant than the peak at 376 nm. When the same film is excited at 390 nm, the peak due to 'band edge' excitonic states is observed at 418 nm. The peak intensities depend on the grown temperature of the material when excited at 250 nm, and the peak intensities

Structural, Optical and Electrical Properties of Undoped and Doped ZnO Thin Films

The Co-doped ZnO thin films show the increase in transmission with a high slope near the fundamental absorption edge in the region of 380–525 nm [1]. The films show high transmittance near the infra-red region. The doping of Co results in the d–d\* intrionic transition in the region from 530 to 692 nm. Moreover, the transmission is 63% when the Co doping concentration is 0 and 79% when the concentration is 4%. The direct and indirect band gap of the Co-doped ZnO thin film is shown in Figure 8. The band gap decreases as the doping concentration

Siagian et al reported the variation of bandgap in Co-doped ZnO films up to the concentration of 10% [2]. The band gap decreases from 3.337 to 3.099 eV as the doping concentration changes from 0 to 10%, and it is shown in Figure 9. The transmittance of the films increases from 68.5 to 83.5% and then decreases as the doping concentration increases. The maximum transmission is obtained for the doping concentration of 7%. Surface roughness, oxygen deficiency and impurity centres are the reasons for a decrease in transmittance when the doping concentra-

More than 90% of transmittance in the visible region is obtained when Fe and Ga is doped in ZnO thin films [25]. As compared with the undoped ZnO films, Fe doping doesn't change the band gap significantly, but Ga doping increases the band gap. The effect of Ni doping in ZnO on its optical properties is reported by Yilmaz [27]. All the films have a sharp absorption edge at 370 nm. The films show high transparency in the region 550 nm and above. The band gap of the materials is found using dT/dλ and Tauc's plot. The transmission spectra and dT/dλ as a function of wavelength is shown in Figure 10. The bandgap of the material decreases as the doping of Ni increases. The transmission and band gap for various Ni doping concentration is given in Table 2. But according to the work published by

remain almost constant when excited at 390 nm.

DOI: http://dx.doi.org/10.5772/intechopen.88905

of Co increases.

Figure 8.

23

'Co' doping concentration vs. band gap.

tion of Co is greater than 7%.

Table 1.

Crystallites size of 'Al'-doped ZnO films.

Figure 7. XRD pattern of IFZO, IAZO and IZO [18].

undoped films and has a negligible intensity as the concentration of 'Al' increases. The crystallite size of the films varies irregularly as the doping of 'Al' concentration changes, and the crystallite sizes are given in Table 1.

Recently, co-doped ZnO (In-Al-co-doped ZnO and In-F-doped ZnO) films are prepared by spray pyrolysis technique. Figure 6 shows the XRD pattern of In-Al- co-doped ZnO (IAZO) and In-F-doped ZnO (IFZO) as compared with In-doped ZnO (IZO) [18].

IFZO films showed a high intensity of (002) diffraction peak compared with other peaks. In addition, IAZO films show only the orientation from (002) peak, which indicates the IAZO films have high stoichiometry than IFZO films. The fullwidth at half-maximum of the IAZO films corresponding to the miller plane (002) is higher than IFZO films indicating that the IAZO has very low grain size than IFZO. This shows that not only the physical method but also chemical synthesis methods tailoring the structural properties of ZnO thin films with ease by altering parameters or by doping is feasible (Figure 7).

#### 3. Optical properties

ZnO films were grown on p<sup>+</sup> -Si substrates prepared by atomic layer deposition (ALD) [17]. The photoluminescence spectrum shows the peaks at 376, 426 and 500 nm when it is excited at 250 nm. The peaks at 376, 426 and 500 nm correspond

#### Structural, Optical and Electrical Properties of Undoped and Doped ZnO Thin Films DOI: http://dx.doi.org/10.5772/intechopen.88905

to the band gap 3.3 eV, 'band edge' excitonic states and reflections of the secondorder harmonic of the excitation source, respectively. Apart from the second-order harmonic peak, the peak 'band edge' excitonic state is dominant than the peak at 376 nm. When the same film is excited at 390 nm, the peak due to 'band edge' excitonic states is observed at 418 nm. The peak intensities depend on the grown temperature of the material when excited at 250 nm, and the peak intensities remain almost constant when excited at 390 nm.

The Co-doped ZnO thin films show the increase in transmission with a high slope near the fundamental absorption edge in the region of 380–525 nm [1]. The films show high transmittance near the infra-red region. The doping of Co results in the d–d\* intrionic transition in the region from 530 to 692 nm. Moreover, the transmission is 63% when the Co doping concentration is 0 and 79% when the concentration is 4%. The direct and indirect band gap of the Co-doped ZnO thin film is shown in Figure 8. The band gap decreases as the doping concentration of Co increases.

Siagian et al reported the variation of bandgap in Co-doped ZnO films up to the concentration of 10% [2]. The band gap decreases from 3.337 to 3.099 eV as the doping concentration changes from 0 to 10%, and it is shown in Figure 9. The transmittance of the films increases from 68.5 to 83.5% and then decreases as the doping concentration increases. The maximum transmission is obtained for the doping concentration of 7%. Surface roughness, oxygen deficiency and impurity centres are the reasons for a decrease in transmittance when the doping concentration of Co is greater than 7%.

More than 90% of transmittance in the visible region is obtained when Fe and Ga is doped in ZnO thin films [25]. As compared with the undoped ZnO films, Fe doping doesn't change the band gap significantly, but Ga doping increases the band gap. The effect of Ni doping in ZnO on its optical properties is reported by Yilmaz [27]. All the films have a sharp absorption edge at 370 nm. The films show high transparency in the region 550 nm and above. The band gap of the materials is found using dT/dλ and Tauc's plot. The transmission spectra and dT/dλ as a function of wavelength is shown in Figure 10. The bandgap of the material decreases as the doping of Ni increases. The transmission and band gap for various Ni doping concentration is given in Table 2. But according to the work published by

Figure 8. 'Co' doping concentration vs. band gap.

undoped films and has a negligible intensity as the concentration of 'Al' increases. The crystallite size of the films varies irregularly as the doping of 'Al' concentration

Recently, co-doped ZnO (In-Al-co-doped ZnO and In-F-doped ZnO) films are prepared by spray pyrolysis technique. Figure 6 shows the XRD pattern of In-Al- co-doped ZnO (IAZO) and In-F-doped ZnO (IFZO) as compared with In-doped

IFZO films showed a high intensity of (002) diffraction peak compared with other peaks. In addition, IAZO films show only the orientation from (002) peak, which indicates the IAZO films have high stoichiometry than IFZO films. The fullwidth at half-maximum of the IAZO films corresponding to the miller plane (002) is higher than IFZO films indicating that the IAZO has very low grain size than IFZO. This shows that not only the physical method but also chemical synthesis methods tailoring the structural properties of ZnO thin films with ease by altering

(ALD) [17]. The photoluminescence spectrum shows the peaks at 376, 426 and 500 nm when it is excited at 250 nm. The peaks at 376, 426 and 500 nm correspond


changes, and the crystallite sizes are given in Table 1.

Crystallite size from topographical analysis (nm)

 26.0 20.9 27.9 16.4 33.7 14.0 31.5 16.4

Crystallite size corresponds to (002) from XRD (nm)

parameters or by doping is feasible (Figure 7).

ZnO (IZO) [18].

Figure 7.

'Al'

2D Materials

Table 1.

concentration

Crystallites size of 'Al'-doped ZnO films.

XRD pattern of IFZO, IAZO and IZO [18].

3. Optical properties

22

ZnO films were grown on p<sup>+</sup>

Figure 9. 'Co' doping concentration vs. band gap.

with undoped ZnO. The near band emission is observed at 3.22 eV when Y concentration is 0% and 3.30 eV when Y is 5%. The Y creates a screened Coulomb potential

Carrier concentration 10.01 <sup>10</sup>21/cm3 27.12 1021/cm3 153.98 1021/cm3 Refractive index 2.34 2.33 2.32

Carrier concentration and refractive index of Sr-doped films compared with undoped ZnO films.

Structural, Optical and Electrical Properties of Undoped and Doped ZnO Thin Films

DOI: http://dx.doi.org/10.5772/intechopen.88905

The band gap increases with an increase in Al concentration in ZnO films [29]. It leads to shifting of absorption band to UV region due to Burstein-Moss shift. The transmittance of doped and undoped ZnO films increase with wavelength. It has a transmittance of 74% in the blue region and more than 90% in the IR region. The decrease in optical transmittance for Al-doped ZnO, when compared with ZnO, is due to the reduction of grain boundaries. The refractive index and extinction coefficient also decreases due to the doping of 'Al'. The transmission of Sr-doped ZnO thin film is higher than undoped ZnO films [16]. Increasing the molarity of the dopant solution increases the transmission coefficient. The optical band gap and the carrier concentration increases, but the refractive index decreases, and the results

ZnO ZnO:Sr (0.1 mM) ZnO:Sr (1 mM)

IZO, IAZO and IFZO films show high transmittance between 70 and 85% in the visible region. The annealing process decreases the transmission for IZO and IAZO films, whereas the transmission increases due to the annealing in the case of IFZO thin films. Moreover, the annealing results in a slight blue shift of the absorption edge. Figure 11 shows the transmission spectra of as-deposited and annealed IZO,

ZnO/Si heterojunction diodes show the maximum rectification for 80°C grown

ZnO, which has the highest rectification [17]. Such junction has fast ON/OFF

field, and the results decrease in the intensity of the near band emission.

are given in Table 3.

Table 3.

Figure 11.

Transmittance spectra [18].

IAZO and IFZO films.

25

4. Electrical properties

Figure 10.

(a) Transmittance spectra and (b) plot of dT/dλ as a function of wavelength [27].


#### Table 2.

Transmittance and band gap of Ni-doped ZnO films.

Karunakaran et al., the addition of Ni in Zn lattice increases the band gap [28]. The addition of Ni increases the refractive index and the extinction coefficient.

Y-doped ZnO films show no deep-level emission but show a strong near band edge emission which is due to the recombination of free excitons in the photoluminescence spectrum [26]. The films have a blue shift to higher energy as compared

Structural, Optical and Electrical Properties of Undoped and Doped ZnO Thin Films DOI: http://dx.doi.org/10.5772/intechopen.88905


Table 3.

Carrier concentration and refractive index of Sr-doped films compared with undoped ZnO films.

Figure 11. Transmittance spectra [18].

with undoped ZnO. The near band emission is observed at 3.22 eV when Y concentration is 0% and 3.30 eV when Y is 5%. The Y creates a screened Coulomb potential field, and the results decrease in the intensity of the near band emission.

The band gap increases with an increase in Al concentration in ZnO films [29]. It leads to shifting of absorption band to UV region due to Burstein-Moss shift. The transmittance of doped and undoped ZnO films increase with wavelength. It has a transmittance of 74% in the blue region and more than 90% in the IR region. The decrease in optical transmittance for Al-doped ZnO, when compared with ZnO, is due to the reduction of grain boundaries. The refractive index and extinction coefficient also decreases due to the doping of 'Al'. The transmission of Sr-doped ZnO thin film is higher than undoped ZnO films [16]. Increasing the molarity of the dopant solution increases the transmission coefficient. The optical band gap and the carrier concentration increases, but the refractive index decreases, and the results are given in Table 3.

IZO, IAZO and IFZO films show high transmittance between 70 and 85% in the visible region. The annealing process decreases the transmission for IZO and IAZO films, whereas the transmission increases due to the annealing in the case of IFZO thin films. Moreover, the annealing results in a slight blue shift of the absorption edge. Figure 11 shows the transmission spectra of as-deposited and annealed IZO, IAZO and IFZO films.

#### 4. Electrical properties

ZnO/Si heterojunction diodes show the maximum rectification for 80°C grown ZnO, which has the highest rectification [17]. Such junction has fast ON/OFF

Karunakaran et al., the addition of Ni in Zn lattice increases the band gap [28]. The

Y-doped ZnO films show no deep-level emission but show a strong near band edge emission which is due to the recombination of free excitons in the photoluminescence spectrum [26]. The films have a blue shift to higher energy as compared

addition of Ni increases the refractive index and the extinction coefficient.

(a) Transmittance spectra and (b) plot of dT/dλ as a function of wavelength [27].

Ni doping % Transmittance at 550 nm (%) Band gap

 90 3.30 3.27 89 3.30 3.26 88 3.29 3.23 85 3.28 3.22 80 3.27 3.19

dT/dλ (eV) Taue's plot (eV)

Figure 9.

2D Materials

Figure 10.

Table 2.

24

Transmittance and band gap of Ni-doped ZnO films.

'Co' doping concentration vs. band gap.

switching ratio up to 103 times/s. When ZnO is prepared at high temperature, the resistivity of the films becomes comparable to the resistivity of the Si substrates. There is no proper variation observed as a function of the preparation temperature of the films. But as the input wavelength of the photon increases, the photoresponsivity increases. Table 4 gives the photoresponsivity of the ZnO/Si heterojunction for various grown temperatures and various wavelengths of the incident photon at 0.5 V reverse bias condition.

The Co-doped ZnO thin films show the semiconducting nature, and it is confirmed from the relationship between the conductivity and temperature [1]. The conductivity increases as the temperature increases. The conductivity is measured from 340 K, not from room temperature. The non-linear behaviour of the electrical conductivity is due to the lattice defects. The activation energy decreases due to the increase in the donor carrier density as the doping concentration of Co increases in the temperature limit of 363–403 K. But the activation energy increases due to decrease in Fermi level as the doping concentration increases in the temperature limit 408–473 K. The reported activation energy is given in Table 5.

In the case of Y-doped ZnO thin films, the electrical resistivity of the film first decreases and then increases as the doping concentration of Y increases [26]. The minimum electrical resistivity of the films is 7.25 ohm-cm, and this value corresponds to the doping concentration of 0.5%. Due to the scattering from grain boundaries and ionized impurities, the Hall mobility decreases gradually from 15.6 to 6.1 cm2 V<sup>1</sup> s 1 . The carrier concentration of both IAZO and IFZO films are higher than IZO films [18]. This is due to the substitution of fluorine ions at oxygen ion site and aluminium ions at zinc site resulting in one free electron per site. Hence the conductivity of both films increases than IZO films. IFZO films have the highest mobility, and IAZO films have the lowest mobility (Figure 12).

5. Conclusion

Figure 12.

Author details

Coimbatore, India

27

Lourdhu Bruno Chandrasekar<sup>1</sup>

T. Daniel Thangadurai<sup>4</sup>

This chapter provides an insight into the property tailoring by parameter variations and doping that gives interesting variation in low dimensions for ZnO. Interesting basic properties and wide range of applications encourage the research about

undoped and doped ZnO thin film synthesis by both physical and chemical methods. They provide amazing opportunity to include a design with ease to prepare ZnO thin film structures possessing desired electrical and optical properties. Representative works by the author group and few others are reviewed to indicate the variation in structural, optical and electrical properties of undoped and metal-

\*, S. Nagarajan<sup>2</sup>

3 Department of Physics, Alagappa Government Arts College, Karaikudi, India

© 2019 The Author(s). Licensee IntechOpen. This chapter is distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/ by/3.0), which permits unrestricted use, distribution, and reproduction in any medium,

4 Department of Nanotechnology, Sri Ramakrishna College of Engineering,

, Marimuthu Karunakaran<sup>3</sup> and

doped ZnO thin films. The co-doped ZnO films are also discussed.

Mobility, conductivity and carrier concentration of IZO, IAZO and IFZO films [18].

Structural, Optical and Electrical Properties of Undoped and Doped ZnO Thin Films

DOI: http://dx.doi.org/10.5772/intechopen.88905

1 Department of Physics, The American College, Madurai, India

\*Address all correspondence to: brunochandrasekar@gmail.com

provided the original work is properly cited.

2 Department of Chemistry, NIT, Imphal, Manipur, India


#### Table 4.

Photoresponsivity of the ZnO/Si heterojunction.


#### Table 5.

Activation energy of Co-doped ZnO films.

Structural, Optical and Electrical Properties of Undoped and Doped ZnO Thin Films DOI: http://dx.doi.org/10.5772/intechopen.88905

Figure 12. Mobility, conductivity and carrier concentration of IZO, IAZO and IFZO films [18].
